Plate thickness/V-groove width | Cold rolled steel plate, galvanized steel plate or aluminum zinc coated steel plate | |||||||||||||
---|---|---|---|---|---|---|---|---|---|---|---|---|---|---|

0.6 | 0.8 | 1.0 | 1.2 | 1.5 | 20 | 2.5 | 3.0 | 3.5 | .0 | 4.5 | 5.0 | Minimum size | remarks | |

V4 | 0.9 | 1.4 | 2.8 | When the part graphic size is marked with a negative tolerance, the bending allowance value can be increased. For example, the red part in the table can be increased by at least: 2.8:2.82,3.4:3.43 or 3.44, 4.5:4.6, 5.5:5.6 | ||||||||||

V6 | 1.5 | 1.7 | 2.0 | 4.5 | ||||||||||

V7 | 1.8 | 2.1 | 2.4 | 5 | ||||||||||

V8 | 1.9 | 2.2 | 2.5 | 5.5 | ||||||||||

V10 | 2.1 | 2.3 | 2.7 | 7 | ||||||||||

V12 | 2.2 | 2.5 | 2.8 | 3.4 | 8.5 | |||||||||

V14 | 3.5 | 3.8 | 6.4 | 6.8 | 10 | |||||||||

V16 | 3.1 | 3.8 | 4.5 | 5.0 | 11 | |||||||||

V18 | 3.3 | 4.0 | 13 | |||||||||||

V20 | 4.0 | 4.9 | 5.1 | 6.6 | 7.2 | 7.8 | 14 | |||||||

V25 | 4.4 | 5.0 | 5.5 | 6.8 | 7.8 | 8.3 | 17.5 | |||||||

V32 | 5.0 | 5.5 | 6.1 | 8.7 |

Cold rolled steel plate, galvanized steel plate or aluminum zinc coated steel plate

Angle | Mold slot width | 90° | Internal bending angle | External bending angle | 180° |
---|---|---|---|---|---|

Plate thickness mm |
|||||

1.5 | V10 | 3 | 3.2 | 4.1 | 0.75 |

2.0 | V12 | 3.84 | 3.7 | 4.6 | 1.0 |

2.5 | V16 | 45 | 4.8 | 6.1 | 1.25 |

Plate thickness mm |
30 | 45° | 60° | 120° | 135 | 145° |
---|---|---|---|---|---|---|

1.0 | 0.35 | 0.7 | 1.1 | 1.0 | 0.6 | 0.4 |

1.2 | 0.4 | 0.8 | 1.2 | 1.0 | 0.6 | 0.4 |

1.5 | 0.5 | 1.0 | 1.6 | 1.4 | 0.9 | 0.6 |

2.0 | 0.6 | 1.2 | 2.0 | 1.7 | 1.1 | 0.7 |

2.5 | 0.8 | 1.6 | 2.6 | 2.2 | 1.4 | 0.85 |

3.0 | 1.0 | 2.2 | 3.4 | 2.8 | 2.0 | 1.2 |

4.0 | 3.7 | 2.4 | 1.4 |

**1.1.1 Example of one-bend unfolding drawing and calculation formula**

- A, B – length of the workpiece bend
- P’ – bending allowance for bend (bending allowance: subtract a allowance for each bend)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + B – P’, i.e., L = 25 + 65 – 5.5 = 84.5

According to Table 1: For a plate thickness of 3 mm, the V25 lower die should be used, with a bending allowance of 5.5.

Note: According to Table 1, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.1.2 Example of two-bend unfolding drawing and calculation formula**

- A(A1), B – length of the workpiece bend
- P – bending allowance for bend (bending allowance: subtract an allowance for each bend)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + T + B – 2xP’, i.e., L = 50 + 2 + 50 – 2×3.4 = 95.6

According to Table 1: For a plate thickness of 2 mm, the V12 lower die should be used, with a bending allowance of 3.4.

Note: According to Table 1, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.1.3. Example of three-bend unfolding drawing and calculation formula**

- A(A1), B(B1) – length of the workpiece bend
- P – bending allowance for bend (bending allowance: subtract an allowance for each bend)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + T + B + T – 3xP’, i.e., L = 50 + 2 + 90 + 2 – 3×3.4 = 133.8

According to Table 1: For a plate thickness of 2 mm, the V12 lower die should be used, with a bending allowance of 3.4.

Note: According to Table 1, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.1.4. Example of four-bend unfolding drawing and calculation formula**

- A, B(B1) – length of the workpiece bend
- P – bending allowance for bend (bending allowance: subtract an allowance for each bend)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + A + B + T + T – 4xP’, i.e., L = 25 + 25 + 100 + 1.5 + 1.5 – 4×2.8 = 141.8

According to Table 1: For a plate thickness of 1.5 mm, the V12 lower die should be used, with a bending allowance of 2.8.

**1.1.5. Example of six-bend unfolding drawing and calculation formula**

- A(A1), B(B1) – length of the workpiece bend
- P’ – bending allowance for bend (bending allowance: subtract an allowance for each bend)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + T + A + T + B + B1 + B1 – 6xP’, i.e., L = 50 + 1.5 + 50 + 1.5 + 150 + 20 + 20 – 6×2.8 = 276.2

According to Table 1: For a plate thickness of 1.5 mm, the V12 lower die should be used, with a bending allowance of 2.8.

**1.2.1. Examples and Calculation Formulas for 180° Bending Unfolding.**

- A, B – length of the workpiece bend
- P – flattening radius bending allowance
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + B – P’, i.e., L = 25 + 65 – 1 = 89

According to Table 2: For a plate thickness of 2 mm, the V12 lower die should be used, with a bending allowance of half the plate thickness.

Note: According to Table 2, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.2.2. Examples and Calculation Formulas for Double-layer Bending Unfolding.**

- A, B – length of the workpiece bend
- P1 – bending allowance for internal corners
- P2 – bending allowance for external corners
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L1 = (A-1.5) + (B-1.5) – P1, i.e., L1 = (65-1.5) + (25-1.5) – 3.2 = 83.8

L2 = A + B – P2, i.e., L2 = 65 + 25 – 4.1 = 85.9

L = L1 + L2 – T/2, i.e., L = 83.8 + 85.9 – 0.75 = 168.95

According to Table 2: For a plate thickness of 1.5 mm, the V12 lower die should be used, with a bending allowance of 3.2 for internal corners, 4.1 for external corners, and 0.75 for a 180° angle.

Note: According to Table 2, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.2.3. Examples and Calculation Formulas for Double-layer Bending Unfolding.**

- A(A1), B1B2- length of the workpiece bend
- P1 – bending allowance for internal angle
- P2 – bending allowance for external angle
- P3 – 90° bending allowance
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness
- P4 – 180°bending allowance

Unfolding length: L1 = A + B1 – P2, i.e., L1 = 75 + 29 – 4.6 = 99.4

L2 = (A1 – T) + (B1 – T) – P1, i.e., L2 = (37 – 2) + (29 – 2) – 3.7 = 58.7

L3 = L1 + L2 – P3, i.e., L3 = 99.4 + 58.3 – 1 = 156.7

L = 25.5 + L3 – P1, i.e., L = 25.5 + 156.7 – 3.84 = 178.36

According to Table 2: For a plate thickness of 1.5 mm, the V12 lower die should be used, with an internal angle bending allowance of 3.2, an external angle bending allowance of 4.1, and a 180° bending allowance of 0.75.

Note: According to Table 2, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.2.4. Examples and Calculation Formulas for Double-layer Bending Unfolding.**

- A, A1, A2, B1, B2, L, L1, L2, L3 – length of the workpiece bend
- P1 – bending allowance for internal angle
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness
- P2 – bending allowance for external angle

Unfolding length: L1 = (A1-T) + (B2-T) – P1, i.e., L1 = (35-2) + (34-2) – 3.7 = 61.3

L2 = (B1-T) + (A2-T) – P1, i.e., L2 = (50-2) + (34-2) – 3.7 = 76.3

L3 = A + B1 + B2 – 2 x P2, i.e., L3 = 70 + 35 + 50 – 2 x 4.6 = 145.8

L = L1 + L2 + L3 – 2 x P3, i.e., L = 61.3 + 75.3 + 145.8 – 2 x 1 = 281.4

According to Table 2: For a plate thickness of 2 mm, the V12 lower die should be used, with an internal angle bending allowance of 3.7, an external angle bending allowance of 4.6, and a 180° bending allowance of 1.

**1.3.1. Examples and Calculation Formulas for Special Angle Bending Unfolding.**

- A(A1), B(B1) – length of the workpiece bend
- P – bending allowance for one-bend angle (varies with the angle)
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = (A-T) + (B-T) – P’ = A1 + B1 – P’, i.e., L = (66-1) + (26-1) – 2 = 65+25-2 = 88

According to Table 3: For a plate thickness of 2 mm, the V12 lower die should be used, and the bending allowance for a 60° angle is 2.

Note: According to Table 3, the neutral layer should be used as the bending length and width.

**1.3.2. Examples and Calculation Formulas for Step Pressing Unfolding.**

- A, B – length of the workpiece bend
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A + 1

Note: When the step is equal to two plate thicknesses, add 0.5 for each step, and add 1 for two steps.

**1.3.3. Examples and Calculation Formulas for Special Angle Unfolding.**

- A(A1A2A3A4), B – length of the workpiece bend
- P – bending allowance for a 135° angle
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Unfolding length: L = A1 + A2 + A3 + A2 + A4 – P – P

Note: For bending with steps, just subtract two allowances.

According to Table 3: For a plate thickness of 2 mm, the V12 lower die should be used, and the bending allowance for a 135° angle is 1.1.

**1.3.4. Examples and Calculation Formulas for Special Angle Unfolding.**

- A(A1A2), B(B1B2) – length of the workpiece bend
- P1 – bending allowance for a 120° angle
- P2 – bending allowance for a 145° angle
- P3 – 90° bending allowance
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness

Note: When the dimension is marked on the outline, it needs to be converted to the neutral layer size when calculating the unfolding length.

Unfolding length: L = A11 + B11 + B21 + A21 – P1 – P2 – P3, i.e., L = 80 + 50 + 103 + 70 – 1.7 – 0.7 – 3.4 = 297.2

According to Table 3: For a plate thickness of 2 mm, the V12 lower die should be used, with a bending allowance of 1.7 for a 120° angle, 0.7 for a 145° angle, and 3.4 for a 90° angle.

Note: According to Table 3, different lower dies have different bending allowances, and different plate thicknesses have different bending allowances.

**1.4.1. Examples and Calculation Formulas for Ordinary Flanging Unfolding.**

- A, B, C – length, width, and height of the workpiece bend
- P – bending allowance
- R – bend radius (usually equal to the thickness of the plate)
- H(H1), L(L1) – unfolding length of each side
- T – material thickness
- D – bending process gap (usually between 0 and 0.5)

Unfolding length: L1 = A, i.e., L1 = 27

L = A + C – P, i.e., L = 27 + 9 – 3.4 = 32.6

H1 = B – T – D, i.e., H1 = 22 – 2 – 0.2 = 19.8 (Note: D is taken as 0.2)

H = B + C – P, i.e., H = 22 + 9 – 3.4 = 27.6

According to Table 1: For a plate thickness of 2 mm, the V12 lower die should be used, with a bending allowance of 3.4.

**1.4.2. Examples and Calculation Formulas for Ordinary Door Flanging Unfolding.**

- A, B, C – length, width, and height of the workpiece bend
- L(L1), H(H1) – unfolding length of each side
- P – bending allowance for a 90° angle
- P1 – bending allowance for a 30° angle
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness
- D – bending process gap (usually between 0 and 0.5)

Unfolding length: L1 = B – T – D, i.e., L1 = 20 – 1.5 – 0.2 = 18.3

L = B + C1 + C2 – P – P1, i.e., L = 20 + 12 + 8.9 – 2.8 – 0.5 = 37.6

H1 = C1 + A – P – D, i.e., H1 = 12 + 35 – 2.8 – 0.2 = 44 (Note: D is taken as 0.2)

H = A + C – P, i.e., H = 35 + 20 – 2.8 = 52.2

According to Table 1: For a plate thickness of 1.5 mm, the V12 lower die should be used, with a bending allowance of 2.8 for a 90° angle and 0.5 for a 30° angle.

**1.4.3. Examples and Calculation Formulas for Ordinary Flanging Bending and Unfolding.**

- A, B, C – length, width, and height of the workpiece bend
- P – bending allowance
- R – bend radius (usually equal to the thickness of the plate)
- T – material thickness
- D – bending process gap (usually between 0 and 0.5)

Unfolding length: H1 = B – B1 – D, i.e., H1 = 50 – 12 – 0.3 = 37.7 (Note: D is taken as 0.2)

H2 = B – T – D, i.e., H2 = 50 – 2.5 – 0.3 = 47.2

H = B + C + B1 – 2xP, i.e., H = 50 + 47 + 12 – 2×4.5 = 100

L1 = A + C – T – D – P, i.e., L1 = 55 + 47 – 2.5 – 0.3 – 4.5 = 94.7

L = A + C+ B2 – 2xP, i.e., L = 55 + 47 + 12 – 2×4.5 = 105

According to Table 1: For a plate thickness of 2.5 mm, the V16 lower die should be used, with a bending allowance of 4.5.

Take your metalworking to the next level with our high-performance machines.

Contact us for a **FREE quote** and see how we can help your projects succeed.

Stay up to date with new and exciting content on various topics, including useful tips.

1. Introduction To meet the large demand for irregular sheet metal in mass production processes of contemporary industrial machinery enterprises, [...]

In today’s rapidly growing industrial market, the demand for reliable and efficient press brakes continues to rise. As an individual [...]

Are you tired of dealing with frustrating faults in your CNC press brake? Do you find yourself constantly troubleshooting and [...]

Contact Us

Our sales engineers are readily available to answer any of your questions and provide you with a prompt quote tailored to your needs.

You will get our expert reply within 24 hours.